High-velocity instabilities in the vortex lattice of Nb/permalloy bilayers
A. Angrisani Armenio,1C. Bell,2J. Aarts,2and C. Attanasio1
1Laboratorio Regionale SuperMat, CNR-INFM Salerno, and Dipartimento di Fisica “E. R. Caianiello,” Università degli Studi di Salerno, Baronissi, Salerno I-84081, Italy
2Kamerlingh Onnes Laboratory, Leiden University, P.O. Box 9504, 2300 RA Leiden, The Netherlands
共Received 13 April 2007; revised manuscript received 11 June 2007; published 1 August 2007兲 We have studied the critical current densityJcfor onset of vortex motion and the dynamic instability of the moving vortex lattice at high driving currents in superconducting共S兲/ferromagnetic共F兲Nb/ Ni0.80Fe0.20 bilay-ers and in a single Nb film with the same thickness. The samples are all characterized by relatively high values of the pinning strength. The measured current-voltage characteristics are successfully described in the frame-work of the Larkin-Ovchinnikov model, modified in order to take into account the effect of the pinning close to the instability. We find thatJcis smaller in the S/F bilayers than in the single film and argue that this is due to the strongly inhomogeneous order parameter in the bilayers. Also, the critical velocityv*for the occurrence of the instability is found to be significantly larger in the S/F bilayers than in the single S layer. By extracting the quasiparticle energy relaxation rate fromv*, we show that this effect is due to the same inhomogeneous order parameter and the resulting lower average value of the superconducting gap.
DOI:10.1103/PhysRevB.76.054502 PACS number共s兲: 74.45.⫹c, 74.78.⫺w, 74.78.Fk
The interplay between a superconductor 共S兲and a ferro-magnet共F兲through the proximity effect in artificial S/F hy-brids is currently a very active field of research involving both fundamental and application aspects.1One of the pecu-liarities of S/F hybrids is the strongly inhomogeneous nature of the superconducting order parameter. On the F side of the interface, the interaction of the exchange field with the Coo-per pairs causes the order parameter to oscillate,1,2 whereas on the S side, the order parameter is strongly suppressed over a distance of the order of the superconducting coherence length S, which is usually a few nanometers. The best known consequences of this highly inhomogeneous character of the order parameter are the strong suppression of the su-perconducting critical temperature Tc with decreasing S-layer thicknessdS, and the nonmonotonic behavior ofTcas function of the thicknessdF of the F layer,3while in S/F/S Josephson junctions, negative critical currents appear.4,5The nonhomogeneous character of the order parameter was also recently studied by measuring the depairing current density
Jdp, which is determined by an average of the superconduct-ing order parameter over the layer thickness.6,7
Such averaging should manifest itself also in other prop-erties of the bilayer system. For instance, the force to pin vortices in the superconductor can be expected to be differ-ent, which is observable by measuring the onset of voltage at the so-called critical current in the current 共I兲-voltage 共V兲
characteristic. Differences should also be found in behavior of the moving vortex system. In particular, at high vortex velocities, an instability can occur, which drives the system to the normal state and therefore manifests itself by a jump in the voltage. This instability, first described by Larkin and Ovchinnikov共LO兲,8is related to the inelastic relaxation rate Eof quasiparticles inside the vortex core. Such instabilities have been observed in a number of systems including low-temperature9–12 and high-temperature superconducting thin films13–16and multilayers.17–19What essentially emerges
from these studies is that the voltage jumps are indeed due to intrinsic properties of the moving vortex lattice but that two more ingredients may play a role,共i兲the temperature depen-dence ofE, in particular, when electron-electron interactions dominate the relaxation, and 共ii兲 vortex pinning, ignored in the original LO theory.20 The LO theory has been also ex-tended to explicitly consider the contributions due to the heating effect.21Finally, measurements of flux-flow instabili-ties have been recently used to extract information about the symmetry of the order parameter in YBa2Cu3O7 thin films.22,23
In the present paper, we study LO instabilities in S/F bi-layers of Nb/ Ni0.80Fe0.20, and for comparison in a single Nb film, by measuring theirI-V characteristics in perpendicular magnetic fields. Using Ni0.80Fe0.20 共Permalloy兲, a strong fer-romagnet, ensures that the order parameter is strongly sup-pressed at the interface, so that the effects of the inhomoge-neous order parameter can be investigated. The outline of the paper is as follows. First, we give the theoretical framework to describe and analyze the flux-flow instabilities, followed by some experimental details. Results are then presented on the critical current densityJcfor the onset of vortex motion and on the critical velocity v* where the instability occurs. From the analysis of the instabilities as a function of the temperature and magnetic field, we establish the role played by the ferromagnet in determining the nonequilibrium Nb properties.
II. VORTEX LATTICE INSTABILITIES
In the case of a vortex lattice moving under high applied driving currents, Larkin and Ovchinnikov theoretically pre-dicted a sudden voltage jump in theI-Vcurves before reach-ing the value of the depairreach-ing currentIdp.8 This fact is im-portant not only from a fundamental point of view but it has also practical implications because it establishes a limit for the sustainable current in the superconducting state. The abrupt switching of the sample to a state of higher electrical
resistance is caused by the electric field generated by the vortex motion, which shifts the distribution of quasiparticles inside the core to higher energies, causing some of them to leave the core all together. The vortex core therefore shrinks with increasing flux-line velocityv, and the viscous damping coefficient decreases. For a critical value of the velocityv*, the flux-flow state becomes unstable and the system switches to the normal state. The amount of decrease of the damping is controlled by the energy relaxation time of the quasiparti-clesE. For the viscous damping coefficientas function of the vortex velocityv, LO obtained the expression
1 +共v/v*兲2, 共1兲
where共0兲is the viscous damping coefficient at zero veloc-ity. From Eq.共1兲, one sees that the damping force Fv=v increases with increasing velocity until it reaches a maxi-mum at v=v*. Since v is proportional to the voltage V
through the Lorentz force, the current-voltage characteristics are, according to LO, described by the relation
1 +共V/V*兲2+cV共1 −t兲
c兲Rf f, 共2兲
wheret=T/Tc is the reduced temperature, Ic is the critical current,Rf f is the flux-flow resistance, andcis a constant of the order of unity. The curve starts to bend upward in the vicinity of the critical voltageV*, which is related tov* by means of the relation
whereHis the applied magnetic field and L is the distance between the voltage contacts.
For the critical velocity LO found
共E兲1/2 , 共4兲
where共x兲is the Riemann zeta function andDis the quasi-particlediffusion coefficient, which means that from measur-ing the critical voltageV*it is possible to estimate values for E. As can be expected, faster relaxation共smallerE兲leads to largerv*. In this respect, it is important to note that a tem-perature dependence can also be expected forE. If the domi-nant relaxation mechanism is electron-phonon scattering, it should be E⬀T−3, while if electron-electron interactions dominate, it isE=E,elexp关2⌬共T兲/kBT兴, whereE,elis basi-cally the inelastic relaxation time of the electron system, and ⌬共T兲 has the temperature dependence ⌬共T兲=⌬共0兲共1 −T/Tc兲1/2 from the BCS theory. This exponential behavior for E was indeed found in various materials, with ⌬共0兲 = 1.76kBTc as expected from the BCS theory for low-Tc amorphous Mo3Si and ⌬共0兲= 3.5kBTc for high-Tc YBa2Cu3O7 共Ref.14兲 in accordance with the enhanced gap values in high-Tc materials. In Ta/ Ge multilayers, again ⌬共0兲= 1.76kBTc was found when the Ta layers were un-coupled, while a coupled anisotropic multilayer yielded ⌬共0兲= 3.5kBTc,18 indicating that the anisotropy leads to an
effective value for ⌬共0兲 without changing the exponential dependence.
Another point to note is that in the LO theory, the critical velocity 关Eq. 共4兲兴 should not be dependent on the external magnetic field.8However, it was discussed that the LO con-dition for a spatially homogeneous quasiparticle nonequilib-rium distribution is only met when the distancev*Eis larger than the intervortex distancea0. At low magnetic fields, this is not the case, andv*becomes proportional toa0and there-fore to
冑1 /H.14The crossover between the two regimes takes place when
v*E=a0f共T兲, 共5兲 wheref共T兲 is a numerical factor of the order of unity.
A Nb film and Nb/Py bilayers were prepared by dc sputter deposition on oxidized Si共100兲 substrates in an ultrahigh vacuum system.24We studied one single 25 nm thick Nb film and two bilayers with the same Nb thicknessdNb= 25 nm and Py thickness dPy= 10 and 75 nm, respectively. As we will see, in all samples, the pinning is relatively high, with the low-field critical current density values higher than 109A / m2 at t=T/Tc= 0.5. Py, apart from having a quite large spin polarization25 is characterized by very small val-ues of the coercive fields Hc at low temperatures, slightly dependent on thickness. Typical values for Hc in our samples, measured with an in-plane field, are around 2 mT
共10 mT兲 for 50 nm共20 nm兲 thick Py films.26 The low
coer-civity, the preferential in-plane magnetization, and the very small thickness make that domain configurations or flux variations in the superconductor due to the ferromagnet do not play a role in our experiments, which are carried out in perpendicular applied field. Even a small in-plane field, for instance, due to external stray fields or a small misalignment of the sample normal with respect to the applied field, will drive out the domains and make the in-plane magnetization uniform. The large demagnetization factor then ascertains that the amount of flux produced by the small volume of the ferromagnetic layer is negligible; in other words, the mag-netic induction equals the applied field.
the temperature dependence of the perpendicular upper criti-cal magnetic fieldsHc2⬜共T兲were resistively measured in the four contact configuration; the values were extracted from the R共T兲 curves, taking the 90% value of the normal state resistanceRNjust above the transition to the superconducting state. The transition widths, estimated from the temperature difference at 10% and 90% of RN, were typically less than 60 mK at zero field and did not substantially broaden, even in high perpendicular magnetic fields, confirming the high quality of our samples. From the slope of the perpendicular upper critical field,27 it is also possible to estimate the quasiparticle diffusion coefficient D=共4kB/e兲 ⫻共−dHc2⬜/兩dT兩T=Tc兲−1for the single Nb film. Because in lay-ered S/F systems theHc2⬜共T兲 curves shift in a parallel way as a function of the layer thicknesses, the slope of the per-pendicular upper critical field cannot be used directly to de-termineDfor the two Nb/Py bilayers.28,29We will takeDfor Nb for all the calculations. Some characteristic parameters of the measured samples are reported in Table I. Note thatTc for the bilayers has decreased by about 1.5 K, which means that the order parameter, assumed to be close to zero at the interface, has relaxed substantially to the bulk value. We therefore expect it to be inhomogeneous over the full film thickness.
IV. RESULTS AND DISCUSSION
A. Critical currents
In Fig. 1共a兲, the I-V characteristics are shown for the single Nb film att= 0.5 for different values of the external magnetic field between 0.05 and 1.8 T as indicated. Up to a certain value of the magnetic field, the curves exhibit a sud-den jump at a well defined current valueI*, well above the critical current Ic where the onset of voltage occurs. At higher magnetic fields, theI-Vcurves become more smeared and finally the jump disappears. This observation is consis-tent with other results found on different kinds of
supercon-ducting systems.9–19 Very similar behavior is observed for both Nb/Py bilayers. In Fig.1共b兲, we show the I-V curves, also measured att= 0.5, for the NbPy75 sample.
The critical current density Jc=Ic/共wd兲 共d is the sample thickness兲 att= 0.5 for the three samples is shown in Fig.2 as a function of the external magnetic field. The critical cur-rentIcwas defined using a dc voltage criterion of 2V. For all samples,Jcrises quickly when the field is lowered below
Hc2 and becomes more or less constant below Hc2/ 2. At these low fields, where the pinning is individual rather than collective, the values forJcrange from 109A / m2for NbPy75 to 5⫻1010A / m2 for Nb. The pinning is therefore quite strong in comparison, for instance, with amorphous materi-als. Also, the values for the two Nb/Py bilayers are substan-tially smaller than for the single film and we want to argue that this is an immediate consequence of the homogeneous
TABLE I. Characteristic parameters of the measured samples. dNb共dPy兲is the Nb共Py兲layer thickness,Tcis the critical tempera-ture, n is the normal state resistivity measured at T= 10 K,
Hc2⬜共t= 0.5兲 is the value of the perpendicular critical field at the reduced temperature equal to 0.5, andDis the quasiparticle diffu-sion coefficient as determined from theHc2⬜ versus temperature
curve for the single Nb film.
Nb 25 0 8.59
NbPy10 25 10 6.97
NbPy75 25 75 6.72
Nb 7.4 1.75 2.78⫻10−4
NbPy10 2.4 0.75
NbPy75 6.7 0.75
suppression of the order parameter inside the Nb. The single-vortex pinning in superconducting films is due to defects in the crystal lattice which can be pointlike or extended共grain boundaries兲 and which cause local variations in the order parameter. Such defects pin vortices because of the smaller amount of condensation energy which locally has to be paid when the vortex resides there. In the region of homoge-neously suppressed superconductivity, which is basically the whole film, the local energy gain is less, and the pinning consequently weaker. We want to note that this is opposite to what can be expected for a magnetic impurity in the super-conducting matrix. In that case, the local suppression is stronger than that of ordinary defects and the pinning will be stronger, as was indeed found in NbTi wires with Ni and Fe impurities.30 The effect is also opposite to the effect from domain walls in the ferromagnet which can pin a vortex by its flux.31,32
Although not central to the paper, we can also remark that the relatively strong pinning in all samples appears to deter-mine the precise shape of theI-V curves. Equation共2兲, for
I⬎Ic, describes the I-V curves close to the instability only when pinning mechanisms are absent and in high enough fields that the flux-flow resistancefis given by the Bardeen-Stephen limitf=nH/Hc2, withnthe normal state resistiv-ity. To include the effect of low fields and pinning, theI-V
relation should be modified as follows18:
1 +共V/V*兲2 + 1
where␣, ␤, and c are constants and used as fitting param-eters. The constant␣corrects for the low-field flux-flow re-sistance; the other two constants parametrize the correction to the viscosity constant by the pinning. In Figs. 3共a兲 and 3共b兲, we show the initial part of theI-V curves close to the instability, for the Nb film and for the NbPy75 bilayer, re-spectively. The solid lines are the fits to the experimental points obtained by using Eq.共6兲. The fits are good, and the values obtained for the parameter␣are quite small共around 10 or less兲for all the magnetic fields in agreement with the
results reported for high-pinning multilayers.18Also, with the obtained values for␣,␤, andc, the theoretical curves do not show any back bending which results in hysteresis not due to thermal origin in theI-Vcharacteristics.10,18Such hysteresis has been observed on amorphous Mo3Si for which, however, the estimated value for the parameter␣ was equal to 14.10
B. Critical velocities
Next, we come to the analysis of the critical velocities. We interpret the voltageV*corresponding to the value of the currentI*, where the jumps in theI-Vcurves appear, as the LO flux-flow instability at the velocityv*. The values ofv*, as obtained directly from the measuredV*using Eq.共3兲, are plotted as a function ofHfor the single Nb film and for the two Nb/Py bilayers in Figs.4共a兲and4共b兲, respectively. In the insets, the behavior ofv*versusH−1/2att= 0.5 for the three FIG. 2. Critical current density versus perpendicular magnetic
field att= 0.5 for the three analyzed samples.
samples is shown. In both cases, the data in low fields show the critical velocity to be proportional to H−1/2, indicating that thermal effects are not responsible for the observed in-stability. For the Nb film, also the crossover to a field-independentv*is found. For the Nb/Py bilayers, the instabil-ity disappears already at field around 0.15 T, and we cannot detect the crossover. The numbers show that the critical ve-locities in the case of the Nb/Py bilayers are much larger and the instability disappears in this case already at smaller fields because the critical voltageV*is always much closer to VN
共the normal state voltage兲 with respect to what happens in
the single Nb film. Also, no substantial difference appears in the results obtained on the two Nb/Py bilayers. This is prob-ably not surprising since Py is characterized by an induced superconducting coherence length of the order of only 1 nm.33However, as noticed in the literature,12,18,21theH−1/2 dependence ofv*can also be induced by unavoidable Joule heating. In this case, a well defined theoretical expression is predicted for the dissipated powerP*=I*V*as a function of
H/HT.12,15,21Here,I*is the current value where instabilities take place and HT is a characteristic magnetic field where
thermal effects start to strongly influence the flux-flow insta-bilities. We did not find any agreement between theory and experiment for the Nb film, while in the case of both the Nb/Py samples, we get0HT= 0.20 T, implying that thermal heating does not considerably influence the field dependence of the measured critical velocities.
What we believe to be the central point of our measure-ments is the fact that for the two Nb/Py bilayers, the v* values are much larger than for the Nb single film. Looking at Eq. 共4兲, this must reflect in very different values for the relaxation time E for the two systems. In Fig. 5, the tem-perature dependenceE is given of for the single Nb film at two different fields, 0H= 0.45 T above and 0H= 0.20 T below the crossover field to constantv* att= 0.5. The solid lines are the curvesE=E,elexp关m⌬共T兲/kBT兴 withE,eland
m both used as fitting parameters. We obtain E,el= 9.74 ⫻10−11s and m= 1.9 for
0H= 0.45 T and E,el= 6.68 ⫻10−12s andm= 1.8 for
0H= 0.20 T. The dashed lines are the fit to the experimental data using the expression E ⬀T−n, where for both fields we obtain the unphysical value
n= 9 for the exponent. The result tells us that electron-electron scattering dominates the energy relaxation in Nb film and that the temperature dependence is due to that of the gap, with⌬共0兲⬇1.76kBTcas expected from the BCS theory. Moreover, the values for E,elare the right order of magni-tude. Similar findings are obtained for the temperature de-pendence of E in the two Nb/Py bilayers. Figure. 5 also shows the temperature dependence of E for the sample NbPy10 at 0H= 0.15 T. The dashed line refers to the power-law fit to experimental data withn= 5, again unphysi-cal, and the solid line is the exponential fit. In this case, E,el= 2.80⫻10−12s, not very different from the number for the Nb film in 0.2 T. The coefficientm, however, turns out to be equal to 1.0, suggesting that the effective gap experienced by the quasiparticles in their relaxation process is only half of the bulk gap. The much larger共critical兲velocities for vor-tices in the bilayer system therefore appear directly related to FIG. 4. Critical velocity v*versus applied magnetic field at t
= 0.5共a兲for Nb film and共b兲for the two Nb/Py bilayers. Insets:v* versus H−1/2att= 0.5共a兲 for Nb film and 共b兲 for the two Nb/Py bilayers. The solid lines are guides to the eyes to show theH−1/2 proportionality ofv*.
FIG. 5. E temperature dependence for the Nb single film at
0H= 0.45 T and 0H= 0.20 T and for NbPy10 at 0H= 0.15 T. The dashed lines are the fit to the experimental data using the ex-pression E⬀T−n, while the solid lines are the fitting curves
the suppression of the superconducting order parameter in the S layer.
We have studied the I-V characteristics at different per-pendicular magnetic fields and temperatures for a Nb single film and for two Nb/Py bilayers with different Py thick-nesses. Critical currents in Nb/Py samples are much smaller than those measured in the single Nb film. We have also observed sudden jumps in theI-Vcurves due to an instability of the vortex lattice which could not be ascribed to heating
effects of the samples. The values of the critical velocities connected to the measured instabilities are much larger in Nb/Py with respect to the Nb. The above experimental find-ings are consistently interpreted as an effect of the strong inhomogeneity of the order parameter in the Nb layer when in contact with the ferromagnet.
This work is part of the research program of the “Stich-ting voor Fundamenteel Onderzoek der Materie 共FOM兲,” which is financially supported by the “Nederlandse Organi-satie voor Wetenschappelijk Onderzoek共NWO兲.”
1A. I. Buzdin, Rev. Mod. Phys. 77, 935共2005兲.
2E. A. Demler, G. B. Arnold, and M. R. Beasley, Phys. Rev. B 55, 15174共1997兲.
3I. A. Garifullin, J. Magn. Magn. Mater. 240, 571共2002兲. 4V. V. Ryazanov, V. A. Oboznov, A. Yu. Rusanov, A. V.
Vereten-nikov, A. A. Golubov, and J. Aarts, Phys. Rev. Lett. 86, 2427
5T. Kontos, M. Aprili, J. Lesueur, F. Genet, B. Stephanidis, and R. Boursier, Phys. Rev. Lett. 89, 137007共2002兲.
6C. Cirillo, A. Rusanov, C. Bell, and J. Aarts, Phys. Rev. B 75, 174510共2007兲.
7J. M. E. Geers, M. B. S. Hesselberth, J. Aarts, and A. A. Golubov, Phys. Rev. B 64, 094506共2001兲.
8A. I. Larkin and Yu. N. Ovchinnikov, Sov. Phys. JETP 41, 960
9W. Klein, R. P. Huebener, S. Gauss, and J. Parisi, J. Low Temp. Phys. 61, 413共1985兲.
10A. V. Samoilov, M. Konczykowski, N.-C. Yeh, S. Berry, and C. C. Tsuei, Phys. Rev. Lett. 75, 4118共1995兲.
11C. Villard, C. Peroz, and A. Sulpice, J. Low Temp. Phys. 131, 957共2003兲.
12C. Peroz and C. Villard, Phys. Rev. B 72, 014515共2005兲. 13S. G. Doettinger, R. P. Huebener, R. Gerdemann, A. Kühle, S.
Anders, T. G. Träuble, and J. C. Villegier, Phys. Rev. Lett. 73, 1691共1994兲.
14S. G. Doettinger, S. Kittelberger, R. P. Huebener, and C. C. Tsuei, Phys. Rev. B 56, 14157共1997兲.
15Z. L. Xiao, P. Voss-de Haan, G. Jakob, and H. Adrian, Phys. Rev. B 57, R736共1998兲.
16Z. L. Xiao, P. Voss-de Haan, G. Jakob, Th. Kluge, P. Haibach, H. Adrian, and E. Y. Andrei, Phys. Rev. B 59, 1481共1999兲. 17B. J. Ruck, J. C. Abele, H. J. Trodahl, S. A. Brown, and P. Lynam,
Phys. Rev. Lett. 78, 3378共1997兲.
18B. J. Ruck, H. J. Trodahl, J. C. Abele, and M. J. Geselbracht, Phys. Rev. B 62, 12468共2000兲.
19C. Peroz, C. Villard, A. Sulpice, and P. Butaud, Physica C 222-226, 369共2002兲.
20Z. L. Xiao and P. Ziemann, Phys. Rev. B 53, 15265共1996兲. 21A. I. Bezuglyj and V. A. Shklovskij, Physica C 202, 234共1992兲. 22B. Kalisky, Y. Wolfus, Y. Yeshurun, G. Koren, and R. P.
Hue-bener, Physica C 401, 273共2004兲.
23B. Kalisky, P. Aronov, G. Koren, A. Shaulov, Y. Yeshurun, and R. P. Huebener, Phys. Rev. Lett. 97, 067003共2006兲.
24A. Yu. Rusanov, M. Hesselberth, J. Aarts, and A. I. Buzdin, Phys. Rev. Lett. 93, 057002共2004兲.
25J. S. Moodera, J. Nowak, and R. J. M. van de Veerdonk, Phys. Rev. Lett. 80, 2941共1998兲.
26A. Yu. Rusanov S. Habraken, and J. Aarts, Phys. Rev. B 73, 060505共R兲 共2006兲.
27J. Guimpel, M. E. de la Cruz, F. de la Cruz, H. J. Fink, O. La-borde, and J. C. Villegier, J. Low Temp. Phys. 63, 151共1986兲. 28Z. Radovic, L. Dobrosavljevic-Grujic, A. I. Buzdin, and J. R.
Clem, Phys. Rev. B 38, 2388共1988兲.
29P. Koorevaar, Y. Suzuki, R. Coehoorn, and J. Aarts, Phys. Rev. B 49, 441共1994兲.
30N. D. Rizzo, J. Q. Wang, D. E. Prober, L. R. Motowidlo, and B. A. Zeitlin, Appl. Phys. Lett. 69, 2285共1996兲.
31L. N. Bulaevskii, E. M. Chudnovsky, and M. P. Maley, Appl. Phys. Lett. 76, 2594共2000兲.
32M. Z. Cieplak, X. M. Cheng, C. L. Chien, and H. Sang, J. Appl. Phys. 97, 026105共2005兲.